A simple planestrain solution for functionally graded multilayered isotropic cylinders


 Hillary Nash
 1 years ago
 Views:
Transcription
1 Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The University of Akron, Akron, OH , USA A. K. Roy Air Force Research Laboratory, Materials and Manufacturing Directorate, AFRL/MLBC, 2941 P St., WPAFB, OH , USA (Received April 7, 2006, Accepted July 11, 2006) Abstract. A simple planestrain solution is derived in this paper for the functionally graded multilayered isotropic elastic cylinder under static deformation. The solution is obtained using method of separation of variables and is expressed in terms of the summation of the Fourier series in the circumferential direction. While the solution for order n = 0 corresponds to the axisymmetric deformation, that for n = 2 includes the special deformation frequently utilized in the upper and lower bounds analysis. umerical results for a threephase cylinder with a middle functionally graded layer are presented for both axisymmetric (n = 0) and general (n = 2) deformations, under either the traction or displacement boundary conditions on the surface of the layered cylinder. The solution to the general deformation case (n =2) is further utilized for the first time to find the upper and lower bounds of the effective shear modulus of the layered cylinder with a functionally graded middle layer. These results could be useful in the future study of cylindrical composites where FGMs and/or multilayers are involved. Keywords: elasticity; analytical solution; micromechanics; functionally graded material; fiber/matrix bond; effective modulus; threephase cylinder. 1. Introduction Functionally graded materials (FGMs) are continuously playing an important role in the design of composite structures. Besides their wellknown applications in thermal coatings for high temperature resistance, FGMs can be utilized as transition layers to reduce the sharp contrast of the material properties between the laminates (i.e., Zhu et al. 1996, Yang and Munz 1997). To assist the design of FGMs, various modeling and simulation methods have been proposed, including both numerical and analytical approaches (i.e., Aihara et al. 1998, Jin et al. 2002). While many analytical results have been reported so far, they are mostly associated with plate geometry only (i.e., Pan 2003, Zhong and Shang 2003, Pan and Feng 2005). To the best of the authors Associate Professor, Corresponding author,
2 2 E. Pan and A. K. Roy knowledge, the corresponding FGM cylindrical composite has not been fully investigated except for some simple deformation cases (Horgan and Chan 1999, Alshits et al. 2001, Oral and Anlas 2005). The present study was motivated by recent experimental work on fiber reinforced composites where it was observed that an FGM interface exists between the fiber and the matrix (Lafdi 2005). As such, from the fabrication and design points of view, it would be helpful if one could understand the effect of different FGMs on the distribution of the displacement, strain, and stress. The ability to estimate the effective material property is also an important issue in the corresponding FGM cylindrical composites. In this paper, we first present the general solution for the FGM cylinder layer by virtue of the method of separation of variables where the θdependent solution in the circumferential direction is expressed in terms of the Fourier series. For multilayered FGM cylinders, a system of linear equations are formed, which can be solved for the given boundary conditions. We discuss further in detail the cases which correspond to the axisymmetric deformation (n = 0) and the deformation of order n = 2 which has been frequently used in the upper and lower bounds analysis. We point out that our formulation for the upper and lower bounds of the shear modulus is presented based on a very simple approach associated with the strain energy and can be for both multilayered and FGM cases. As examples, numerical results on the displacement, strain, and stress are presented for the threephase cylinder with a FGM middle layer. The analysis shows clearly the influence of the FGM layer on the field distribution in the inner and outer homogeneous layers as well as in the FGM layer. The corresponding effective shear moduli for the threephase cylinder with FGM middle layer or with homogeneous middle layer are also predicted for the first time based on the solution. Results in this paper could be useful in future numerical study of the layered FGM cylindrical composites based on either boundary or finite element method. The paper is organized as follows: In Section 2, the general solution for the multilayered FGM cylinder is derived based on the method of separation of variables. In Section 3, the upper and lower bounds formulation is presented for the FGM and multilayered cylinder, which is based on the simple energy equivalence in the radical direction only. umerical examples are presented in Section 4 to show the influence of the FGM layer on displacement, strain, and stress fields as well as on the upper and lower bounds. Finally, conclusions are drawn in Section 5. Fig. 1 A threephase FGM composite cylinder
3 A simple planestrain solution for functionally graded multilayered isotropic cylinders 3 2. General solutions for the multilayered FGM cylinder Assume that a layered cylinder consists of L layers, which can be homogeneous or FGM (a threelayered cylinder is shown in Fig. 1). The layered cylinder is solid so that it includes the inner most layer (r = 0) j = 1. For any layer j of the cylinder bounded by r = R j 1, R j (R j > R j 1 ), we assume the Young s modulus as a function of radius in the form of E j r ( r ) E 0j  R where R is a nominal length within the layer j, k is the FGM factor which characterizes the variation of the Young s modulus within the layer, and E 0j is the proportional constant. To find the general solution for each layer, we utilize the method of separation of variables with Fourier series in the θdirection (as a summation from 0 to a large but finite ). In other words, we assume that the displacement, strain, and stress fields can be expressed as k (1) u r ε r ( r, θ ) ε rn ( r )e inθ ( r, θ ) u rn ( r )e inθ ; u θ ( r, θ ) i u θn ( r )e inθ ; ε θ ( r, θ ) ε θn ( r )e inθ ; γ rθ ( r, θ ) i γ rθn r σ r ( r, θ ) σ rn ( r )e inθ ; σ θ ( r, θ ) σ θn ( r )e inθ ; τ rθ ( r, θ ) i τ rθn r ( )e inθ ( )e inθ (2) (3) (4) where i = ( 1), and the shear stress τ rθ is also represented alternatively as σ rθ. We remark that while n = 0 corresponds to the axisymmetric deformation, n = 2 corresponds to the case used most frequently in the upper and lower bounds moduli estimation for threephase composites (i.e., Christensen and Lo 1979, Qiu and Weng 1991). It is emphasized, however, that the solution presented here is more general, which includes multilayered FGMs with the formulation being very simple. For example, in order to solve the general problem in the rθ space, it is sufficient for us to look at the corresponding amplitude of the field quantities for the given order n (or the rdependent function only). Keeping this in mind, the straindisplacement relations and the equilibrium equations in terms of the amplitudes are then reduced to (being functions of the variable r only) ε rn du rn /dr; ε θn u rn /r nu θn /r γ rθn nu rn /r du θn /dr u θn /r dσ rn /dr nτ rθn /r ( σ rn σ θn )/r 0 dτ rθn /dr nσ θn /r 2τ rθn /r 0 (5) (6) The constitutive relation between the stress and strain is similar to the wellknown Hooke s law with the exception that the Young s modulus is now a function of the radius r. Eqs. (5) and (6), combined with the isotropic constitutive relation, can be used to solve the unknown amplitudes of the displacement, strain, and stress fields. More specifically, in order to find
4 4 E. Pan and A. K. Roy the amplitude of the displacement field in each FGM layer, we assume the nth order solution as u rn ( r ) u θn ( r ) c 1 c 2 r p (7) where the unknown factor p and the corresponding coefficients (c 1 and c 2 ) can be solved from the following eigensystem of equations: { 2( k p 1) [( 1 ν j )p ν j ] n 2 ( 1 2ν j ) 21 ( 2ν j )( p 1 )}c 1 { 2ν j n( k p 1) n( 1 2ν j )( p 1) 2n( 1 2ν j )}c 2 0 { n( 1 2ν j )( k p 1 ) 2n( ν j p 1 ν j ) 2n( 1 2ν j )}c 1 {( 1 2ν j )( k p 1 )( p 1) 2n 2 ( 1 ν j ) 21 ( 2ν j )( p 1 )}c 2 0 (8) where ν j is the Poisson s ratio of the layer j, and k again characterizes the FGM as given in Eq. (1). For any layer other than the inner layer (r = 0), there are generally four different (complex) roots p m with four different (complex) pairs of eigenvectors (c 1m, c 2m ) (see Appendix A for detailed discussion). Therefore, the amplitudes of the displacements can be obtained as u rn ( r ) u θn ( r ) 4 c Re b 1m m r pm m 1 c 2m (9) where Re stands for the real part of the complex function. Once the displacement amplitudes are found, amplitudes of the strains are obtained using the displacementstrain relation, and stresses using the constitutive relation. It is obvious that for the solution to be bounded for the inner layer (r = 0), it is necessary to choose solutions corresponding to the two roots which have a positive real part. Once the general solution for each layer is derived, the boundary condition as well as the interface condition can be applied to solve all the unknowns involved in the layered cylinder (assuming continuity of the displacement and traction vectors at the interfaces between adjoining layers). The size of the system of linear equations will be proportional to the number of layers. Alternatively, it is possible to find the propagator matrix for each layer and then propagate the solutions from layer to layer (i.e., Pan 1997) to arrive at a system of equations involving only 2 unknowns. The propagator matrix (or transfer matrix) has been utilized previously in many areas including those related to laminate FGM composites (e.g., Pan 2001, 2003, Pan and Han 2005). In this paper, however, the direct solution method is adopted as the number of layers studied here is relatively small. 3. Upper and lower bounds of the effective shear modulus for multilayered FGM cylinders In this section, we follow the general procedure as in Christensen and Lo (1979) and Qiu and Weng (1991) for threephase composites in order to find both the upper and lower bounds of the effective shear modulus for multilayered FGM cylinders. It can be observed that the formulation
5 A simple planestrain solution for functionally graded multilayered isotropic cylinders 5 presented here is extremely simple with all the calculations in the radial rdirection only. In order to obtain the upper bound, we apply the following displacement condition on the surface of the outer layer r = R L (in terms of the Cartesian coordinates (x 1, x 2 ) in the (r, θ )plane): u α ( r R L ;θ ) ε αβ x β (10) where the described nonzero components of the strain tensor are ε 11 ε 22 ε (11) It is easy to show that in terms of the polar coordinates, the displacement boundary condition becomes u r ( r R L ;θ ) u θ ( r R L ;θ ) ε R L cos2θ sin2θ (12) Or in general, u r ( r R L ;θ ) u θ ( r R L ;θ ) ε R L e 2iθ ie 2iθ (13) Therefore, the displacement amplitudes of second order (n = 2) should satisfy the following boundary condition: u r2 ( r R L ) ε R L (14) u θ2 ( r R L ) Again, the subscript 2 on the lefthand side of the equation indicates the amplitude of the displacement corresponding to order n = 2. Similarly, to find the lower bound, the traction boundary condition on the surface of the outer layer r = R L (again, in terms of the Cartesian coordinates) is described by: t α ( r R L ;θ ) σ αβ n β (15) where the described nonzero components of the stress tensor are σ 11 σ 22 σ (16) In terms of the polar coordinates, the traction boundary condition becomes σ r ( r R L ;θ ) τ rθ ( r R L ;θ ) σ cos2θ sin2θ (17) Or in general, σ r ( r R L ;θ ) τ rθ ( r R L ;θ ) σ e2iθ ie 2iθ (18)
6 6 E. Pan and A. K. Roy Therefore, the corresponding traction amplitudes of order n = 2 satisfy the following boundary condition: σ r2 ( r R L ) τ rθ2 ( r R L ) σ (19) In both cases, the effective shear modulus G eff is calculated based on the equivalence of the strain energies between the multilayered FGM model and the homogeneous model with the effective shear modulus. The derivation is presented below: Since both the multilayered FGM and the homogeneous models have the same θdependence, multiple factors from integration over the variable θ are therefore the same on both sides of the energy equation. Consequently, it is only necessary to carry out the integration along the radial direction. For a linear elastic cylinder made of L FGM layers, the strain energy is calculated from L 1 R E Total j  σ αβ2 ( r )ε αβ2 ( r )rdr 2 R j 1 j L j 1 R j R j 1 2G ν 1 2ν [( )( ε r2 ε θ2 ) 2νε r2 ε θ2 ] Gγ rθ2 rdr (20) This expression can be used to find energy in the multilayered FGM model once all the coefficients in each layer are solved under the given boundary and interface conditions. The energy for the corresponding homogeneous model with the undetermined effective shear modulus G eff is evaluated based on simple surface integration where the θ integration cancels out when equating this expression to that of the multilayered FGM model in Eq. (20). For the equivalent homogeneous model, the total energy is E 1  σ αβ2 ε αβ2 dv σ αβ2 n β u α2 ds 2 Ignoring the θdependent factor, the effective energy is therefore reduced to (21) 1 E eff  σ αβ2 n β u α2 R L (22) 2 Using either the displacement or traction boundary condition, combined with the solved coefficients for the equivalent model, it can be shown that the expression for the effective energy Eq. (22) involves only the effective shear modulus as the unknown. Letting the effective energy Eq. (22) equal the multilayered FGM energy Eq. (20), then the effective shear modulus G eff can be finally solved. 4. umerical examples 4.1 Example 1: Upper and lower bounds of shear modulus in threephase cylinders We first checked our solution of multilayered cylinders for the effective shear modulus. For the
7 A simple planestrain solution for functionally graded multilayered isotropic cylinders 7 Fig. 2 Comparison of the amplitudes (n = 2) of stresses based on the FGM vs. discrete layered models under the displacement boundary condition Table 1 Upper and lower bounds of the effective shear modulus G eff for the threephase composite with ν 1 = ν 2 = ν 3 =0.3 and d 2 :d 1 =2:1 E 1 /E 2 /E 3 Fraction d 1 Upper G eff Lower G eff 1/5/25 25/5/1 25/1/ threephase cylinder case considered in Qiu and Weng (1991), the Young s modulus E i in each layer takes a value of 1, 5, or 25 (for example, E 1 /E 2 /E 3 = 1/5/25 for one of the models), whilst the Poisson s ratio is the same, i.e., ν 1 = ν 2 = ν 3 = 0.3. The upper and lower bounds for the shear modulus predicted from our analytical formulation are found to be the same as those in Qiu and Weng (1991, Figs. 1 and 2). For instance, listed in Table 1 are some of the results from our solution for different volumetric fractions d 1 (with fixed d 2 :d 1 = 2:1). The corresponding radii of the threephase cylinder are given in Table 2.
8 8 E. Pan and A. K. Roy Table 2 Volumetric fraction d 1 and the corresponding radii of the threephase cylinder for fixed ratio d 2 :d 1 =2:1 d 1 R 1 R 2 R Example 2: A threephase cylinder with a middle FGM layer (n = 2) The second example is for a threephase cylinder with a middle FGM layer. Solutions for both the direct FGM and discrete models are employed to carry out the calculation. In the discrete model, a total of 12 layers are used. In other words, 10 discrete homogeneous layers are used to approximate the middle FGM layer (it has been checked that when the number of the discrete layers is equal to 10 or larger, the discretebased solution is nearly the same as the FGM solution). The FGM factor k in Eq. (1) is chosen in such a way that E 2 (r) = (r/r 1 ) in the FGM layer. Other parameters are R 1 = 1.0, R 2 = 2.0, and R 3 = 3.0, ν 1 = ν 2 = ν 3 = 0.3, E 1 = 1 and E 3 = 25. It is obvious that when r = R 1 we have E 2 = 1, and at r = R 2, we have E 2 = 5. The boundary condition applied at R 3 = 3.0 is the displacement condition described by Eq. (14) with ε 1. For example, the amplitudes of the stresses from both the direct FGM and discrete homogeneous models are plotted in Fig. 2. It is observed that both models predict very close results to each other. Furthermore, there is a sharp discontinuity for the normal stress σ θ across the interface at r = 2 due to the jump of the Young s moduli on both sides of the interface. We have also compared this FGM model to a couple of discrete homogeneous threephase models with different combinations of E 1 /E 2 /E 3. While the results for the upper and lower bounds are given in Table 3, the amplitudes of the stress components for different models are presented in Figs. 3(a), 3(b), and 3(c) for the traction boundary condition Eq. (19) with σ 1. It is interesting to note from Table 3 that the shear modulus bounds for the FGM case is somewhere between those of the discrete models E 1 /E 2 /E 3 = 1/2/25 and E 1 /E 2 /E 3 = 1/3/25. From Fig. 3, we first observe that while the normal (σ r ) and shear (τ rθ ) stresses have approximately the same magnitude, the amplitude of the hoop stress σ θ is much larger. For different combinations of E 1 /E 2 /E 3, the stress amplitude could decrease in one layer and increase in another for increasing E 2 in the middle layer. For instance, with increasing E 2, the amplitude of σ r decreases in layers 1 and 2 but increases in layer 3 (Fig. 3(a)). However, the trend for the FGM layer case is different: while the stress variation for the FGM layer model follows the curve of one of the discrete models E 1 /E 2 /E 3 in layers 1 and 3, its behavior in the FGM middle layer is different: It Table 3 Upper and lower bounds of the shear modulus for the FGM middle layer model and the discrete homogeneous models with different combinations of E 1 /E 2 /E 3 E 1 /E 2 /E 3 Upper G eff Lower G eff 1/2/ FGM /3/ /5/
9 A simple planestrain solution for functionally graded multilayered isotropic cylinders 9 Fig. 3 Amplitudes (n = 2) of stresses in FGM and discrete layered cylinders under traction boundary condition: Stress σ r in (a), σ θ in (b), and σ rθ in (c) crosses some (Figs. 3(a) and 3(c)) or all (Fig. 3(b)) of the curves predicted based on the discrete models E 1 /E 2 /E 3 in the middle layer. More importantly, the stress variation in the FGM middle layer is much smoother than those in the homogeneous middle layer, and there is no discontinuity for the stress σ θ across the interface between the FGM and the inner layer as the Young s moduli is continuous there. 4.3 Example 3: A threephase cylinder with a middle FGM layer (n = 0) The effect of different k values in the FGM model (Eq. (1)) is studied in this example, where the
10 10 E. Pan and A. K. Roy Fig. 4 Young s modulus in the middle FGM layer of a threephase cylinder k in the middle FGM layer (1 < r <2) varies as k = 0, 1/2, 1, 2, 3, 4, 5. The deformation is restricted to the axisymmetric case (i.e., n = 0) under uniform traction (i.e., σ r0 (( r R 3 ) 1). While the Poisson s ratios are the same in the three layers (i.e., ν 1 = ν 2 = ν 3 = 0.3), the Young s moduli in the inner layer (r < 1) and outer layer (2 < r < 5) are, respectively, E 1 = 10 and E 3 = 1. The Young s modulus E 2 in the FGM middle layer (1 < r < 2) is described by Eq. (1) with E 02 = 10 and its distribution for different k is plotted in Fig. 4. The corresponding solutions for the displacement, strain, and stress are presented in Figs. 5(a), 5(b), and 5(c). Some interesting features can be observed from Fig. 5: 1) Since the Young s modulus in the inner layer is larger than those in the other two layers, the induced displacement and strain fields in this layer are much smaller. Therefore, the effect of different k values on the displacement and strain fields within layer 1 (r < 1) cannot be clearly observed (Figs. 5(a) and 5(b)). 2) For displacement u r (Fig. 5(a)), its values in both the FGM and outer layers increase with increasing magnitude of k. For strain ε r (Fig. 5(b)), however, with increasing magnitude of k, its value increases in the FGM layer, but decreases in the outer layer. 3) As for the stress in the inner layer, increasing magnitude of k corresponds to an increase of the stress value for k = 0 to 3; however, when k = 4 and 5, the stress amplitude is reduced, with the result for k = 5 close to that for k = 1/2 (Fig. 5(c)). This feature is possibly due to the fact that for k = 0 to 3, the Young s moduli in the FGM layer are all larger than that in the outer layer; however, for k = 4 and 5, they become smaller in the FGM layer than that in the outer layer (near r = 2 in the FGM layer in Fig. 4). 4) In the outer layer, the stress σ r decreases with increasing magnitude of k (Fig. 5(c)). In general, different k values have apparent effect on the displacement, strain, and stress in both the FGM middle layer and the outer layer. While the response (displacement, strain, or stress) as a
11 A simple planestrain solution for functionally graded multilayered isotropic cylinders 11 Fig. 5 Amplitudes (n = 0) of the field quantities for different FGM factors k: Radial displacement u r in (a), strain ε r in (b), stress σ r in (c) function of r is gentle in the outer layer, the one in the FGM layer experiences a large change in its amplitude. It is also obvious that, the transfer of the stress from the inner to the outer layer is more complicated than that of the displacement or strain, with the inner fiber carrying most of the stress. 5. Conclusions In this paper, exact solutions are derived for multilayered FGM cylinders under static deformation. They are obtained based on the method of separation of variables and include the previous
12 12 E. Pan and A. K. Roy axisymmetric solution as a special case. The most commonly used upper and lower bounds formulation is also extended to the general multilayered FGM case and is further presented in terms of a simple energy relation. While our solutions can be applied to many different deformation cases, illustrative results for a threephase cylinder with a FGM middle layer are presented for orders n = 0 and 2. It is observed clearly that the FGM middle layer can strongly influence the field (displacement, strain, and stress) distribution within the FGM layer and in the inner and outer layers as well. The FGM layer also has an obvious effect on the upper and lower bounds of the effective shear modulus. Results presented in this paper could be useful in future numerical analysis of FGM layered cylinders based on the boundary and finite element methods. Acknowledgements This work was carried out while the first author was at AFRL under the Air Force 2005 Summer Faculty Fellowship Program. References Aihara, T. Jr., Sho, T. and Kawazoe, Y. (1998), Molecular dynamics simulation on elastic behavior of i/i 3 Al interface with graded structure, J. Japan Institute of Metals, 62, Alshits, V.I. and Kirchner, H.O.K. (2001), Cylindrically anisotropic, radially inhomogeneous elastic materials, Proc. R. Soc. Lond, A 457, Christensen, R.M. and Lo, K.H. (1979), Solutions for effective shear properties in three phase sphere and cylinder models, J. Mech. Phys. Solids, 27, Horgan, C.O. and Chan, A.M. (1999), The pressurized hollow cylinder or disk problem for functionally graded isotropic linearly elastic materials, J. Elasticity, 55, Jin, Z.H., Paulino, G.H. and Dodds, Jr. R.H. (2002), Finite element investigation of quasistatic crack growth in functionally graded materials using a novel cohesive zone fracture model, J. Appl. Mech., 69, Lafdi, K. (2005), TEM characterization of the interface property between the fibre and matrix, Private Communication. Oral, A. and Anals, G. (2005), Effects of radially varying moduli on stress distribution of nonhomogeneous anisotropic cylindrical bodies, Int. J. Solids Struct., 42, Pan, E. (1997), Static Green s functions in multilayered halfspaces, Applied Mathematical Modelling, 21, Pan, E. (2001), Exact solution for simply supported and multilayered magnetoelectroelastic plates, ASME, J. Appl. Mech., 68, Pan, E. (2003), Exact solution for functionally graded anisotropic elastic composite laminates, J. Composite Mater., 37, Pan, E. and Han, F. (2005), Exact solution for functionally graded and layered magnetoelectroelastic plates, Int. J. Eng. Sci., 43, Qiu, Y.P. and Weng, G.J. (1991), Elastic moduli of thickly coated particle and fiberreinforced composites, J. Appl. Mech., 58, Tarn, J.Q. (2001), Exact solutions for functionally graded anisotropic cylinders subjected to thermal and mechanical loads, Int. J. Solids Struct., 38, Yang, Y.Y. and Munz, D. (1997), Reduction of residual stresses in a two dissimilar materials joint by using a functionally graded material, In Composites and Functionally Graded Materials, Proc. of the Symposia, ASME International Mechanical Engineering Congress and Exposition, Dallas, TX, Zhong, Z. and Shang, E.T. (2003), Threedimensional exact analysis of a simple supported functionally gradient
13 A simple planestrain solution for functionally graded multilayered isotropic cylinders 13 piezoelectric plate, Int. J. Solids Struct., 40, Zhu, J., Yin, Z., Mao, J., Lai, Z., Yang, D., ing, X. and Li, D. (1996), Interface structure of ZrO 2 i functionally gradient material, Acta Metallurgica Sinica, 32, Appendix A: Roots of the eigensystem of Eqs. (8) Using Mathematica, the four different roots p m (m = 1, 2, 3, 4) of the system of Eq. (8) can be found as (for simplicity, the Poisson s ratio in layer j, ν j, has been replaced with ν ): where p 1 4 k ± k a± b ( ν) (A1) a 1 2n 2 ( 1 ν ) 1 k ( )( 1 2ν ) b k 2 16n 2 2 ( 1 ν ) 8n 2 ( k 4ν) 8kn 2 ν( 3 2ν) 4k 2 n 2 ν 1 ν ( ) (A2) We remark that in general the four roots are complex. Therefore, the corresponding eigenvectors (c 1m, c 2m ) are also complex. Since the displacement solution is real, one needs to take only the real part of the complex solution. We discuss below the solutions corresponding to those with special functional gradient k and Poisson s ratio v values: 1) k = 0 This corresponds to the homogeneous material case. For this case, the four roots p m in Eq. (A1) are real, and can be expressed as n± 1 p 1 4 ±( ) (A3) The same roots can also be easily derived from the governing equations when the material is homogeneous. 2) n = 0 This corresponds to the axisymmetric deformation studied in detail in the paper. For the axisymmetric case, the four roots p m are k/2± k 2 /4 k 1; m 1, 2 p m k/2± k 2 /4 k kν/ ( 1 ν ); m 3, 4 It is obvious that for the regular domain of k 0 and 0 ν 1/2, all the roots in Eq. (A4) are real. (A4) 3) n =2 This corresponds to the special deformation associated with the prediction of the effective shear modulus, as discussed in the paper. For this case, a 10( 1 ν ) k 1 2ν b k 2 2 ( 1 16ν 16ν ) 32k 1 2ν ( ) ( ) 1 ν ( ) 64 1 ν ( ) 2 (A5) It is apparent that for n = 2 and also for other orders, the four roots will be, in general, complex (in pair). For example, for ν = 0.3, the four roots are
14 14 E. Pan and A. K. Roy k ± 1.96k k ± k 2.36k 2 p 1 4 ( ) (A6) which, for the special functional gradient k = 3 studied in the paper, become ± i; m 1, 2 p m ± i; m 3, 4 (A7)
The Rotating Inhomogeneous Elastic Cylinders of. VariableThickness and Density
Applied Mathematics & Information Sciences 23 2008, 237 257 An International Journal c 2008 Dixie W Publishing Corporation, U. S. A. The Rotating Inhomogeneous Elastic Cylinders of VariableThickness and
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationStress analysis of functionally graded discs under mechanical and thermal loads
Indian Journal of Engineering & Materials Sciences Vol. 8, April 0, pp. 8 Stress analysis of functionally graded discs under mechanical and thermal loads Hasan Çallioğlu, Metin Sayer* & Ersin Demir Department
More informationA parametric study on the elasticplastic deformation of a centrally heated twolayered composite cylinder with free ends
Arch. Mech., 68, 3, pp. 03 8, Warszawa 06 A parametric study on the elasticplastic deformation of a centrally heated twolayered composite cylinder with free ends F. YALCIN ), A. OZTURK ), M. GULGEC 3)
More informationStresses and Displacements in Functionally Graded Materials of SemiInfinite Extent Induced by Rectangular Loadings
Materials 2012, 5, 210226; doi:10.3390/ma5020210 Article OPEN ACCESS materials ISSN 19961944 www.mdpi.com/journal/materials Stresses and Displacements in Functionally Graded Materials of SemiInfinite
More informationROTATING RING. Volume of small element = Rdθbt if weight density of ring = ρ weight of small element = ρrbtdθ. Figure 1 Rotating ring
ROTATIONAL STRESSES INTRODUCTION High centrifugal forces are developed in machine components rotating at a high angular speed of the order of 100 to 500 revolutions per second (rps). High centrifugal force
More informationTHERMOELASTIC ANALYSIS OF THICKWALLED FINITELENGTH CYLINDERS OF FUNCTIONALLY GRADED MATERIALS
Journal of Thermal Stresses, 28: 391 408, 2005 Copyright # Taylor & Francis Inc. ISSN: 01495739 print/1521074x online DOI: 10.1080/01495730590916623 THERMOELASTIC ANALYSIS OF THICKWALLED FINITELENGTH
More information17th European Conference on Fracture 25 September,2008, Brno, Czech Republic. Thermal Fracture of a FGM/Homogeneous Bimaterial with Defects
5 September,8, Brno, Czech Republic Thermal Fracture of a FGM/Homogeneous Bimaterial with Defects Vera Petrova, a, Siegfried Schmauder,b Voronezh State University, University Sq., Voronezh 3946, Russia
More informationDistributed: Wednesday, March 17, 2004
MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MECHANICAL ENGINEERING CAMBRIDGE, MASSACHUSETTS 019.00 MECHANICS AND MATERIALS II QUIZ I SOLUTIONS Distributed: Wednesday, March 17, 004 This quiz consists
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationMaterial tailoring and moduli homogenization for finite twisting deformations of functionally graded MooneyRivlin hollow cylinders
Acta Mech 224, 811 818 (2013) DOI 10.1007/s007070120784z J. R. Dryden R. C. Batra Material tailoring and moduli homogenization for finite twisting deformations of functionally graded MooneyRivlin hollow
More informationMechanical Properties of Polymer Rubber Materials Based on a New Constitutive Model
Mechanical Properties of Polymer Rubber Materials Based on a New Constitutive Model Mechanical Properties of Polymer Rubber Materials Based on a New Constitutive Model J.B. Sang*, L.F. Sun, S.F. Xing,
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More information3 2 6 Solve the initial value problem u ( t) 3. a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1
Math Problem a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b True or false and why 1. if A is
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationAdvanced Structural Analysis EGF Cylinders Under Pressure
Advanced Structural Analysis EGF316 4. Cylinders Under Pressure 4.1 Introduction When a cylinder is subjected to pressure, three mutually perpendicular principal stresses will be set up within the walls
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES
Advanced Composite Letters, Vol. 9, No. 6, 373383 000 Full Article ANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES John A. Nairn Material
More informationAnalysis of Squareshaped Crack in Layered Halfspace Subject to Uniform Loading over Rectangular Surface Area
Copyright 2015 Tech Science Press CMES, vol.109110, no.1, pp.5580, 2015 Analysis of Squareshaped Crack in Layered Halfspace Subject to Uniform Loading over Rectangular Surface Area H. T. Xiao 1,2,3,
More informationLaminated Composite Plates and Shells
Jianqiao Ye Laminated Composite Plates and Shells 3D Modelling With 62 Figures Springer Table of Contents 1. Introduction to Composite Materials 1 1.1 Introduction 1 1.2 Classification of Composite Materials
More informationMechanical Design in Optical Engineering
Torsion Torsion: Torsion refers to the twisting of a structural member that is loaded by couples (torque) that produce rotation about the member s longitudinal axis. In other words, the member is loaded
More informationInhomogeneity Material Effect on Electromechanical Stresses, Displacement and Electric Potential in FGM Piezoelectric Hollow Rotating Disk
Journal of Solid Mechanics Vol. 2, No. 2 (2010) pp. 144155 Inhomogeneity Material Effect on Electromechanical Stresses, Displacement and Electric Potential in FGM Piezoelectric Hollow Rotating Disk A.
More informationMoving screw dislocations in piezoelectric bimaterials
phys stat sol (b) 38 No 1 10 16 (003) / DOI 10100/pssb00301805 Moving screw dislocations in piezoelectric bimaterials XiangFa Wu *1 Yuris A Dzenis 1 and WenSheng Zou 1 Department of Engineering Mechanics
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationAnalytical Solution for Electromechanical Behavior of Piezoelectric Rotating Shaft Reinforced by BNNTs Under Nonaxisymmetric
Journal of Solid Mechanics Vol. No. () pp. 33935 Analytical Solution for Electromechanical Behavior of Piezoelectric Rotating Shaft Reinforced by BNNTs Under Nonaxisymmetric Internal Pressure A. Ghorbanpour
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationTorsion of Shafts Learning objectives
Torsion of Shafts Shafts are structural members with length significantly greater than the largest crosssectional dimension used in transmitting torque from one plane to another. Learning objectives Understand
More information16.20 HANDOUT #2 Fall, 2002 Review of General Elasticity
6.20 HANDOUT #2 Fall, 2002 Review of General Elasticity NOTATION REVIEW (e.g., for strain) Engineering Contracted Engineering Tensor Tensor ε x = ε = ε xx = ε ε y = ε 2 = ε yy = ε 22 ε z = ε 3 = ε zz =
More informationOn the torsion of functionally graded anisotropic linearly elastic bars
IMA Journal of Applied Mathematics (2007) 72, 556 562 doi:10.1093/imamat/hxm027 Advance Access publication on September 25, 2007 edicated with admiration to Robin Knops On the torsion of functionally graded
More informationfunctionally graded material, piezoelectric material, circular plates, uniform electric potential, direct displacement
Science in China Series G: Physics, Mechanics & Astronomy 008 SCIENCE IN CHINA PRESS SpringerVerlag www.scichina.com phys.scichina.com www.springerlink.com Threedimensional analytical solution for a
More informationFree Vibration Analysis of Functionally Graded Material Plates with Various Types of Cutouts using Finite Element Method
International Journal of Current Engineering and Technology EISSN 2277 4106, PISSN 2347 5161 2018 INPRESSCO, All Rights Reserved Available at http://inpressco.com/category/ijcet Research Article Free
More informationMechanics PhD Preliminary Spring 2017
Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationRayleigh waves in magnetoelectroelastic half planes
Acta Mech 202, 127 134 (2009) DOI 10.1007/s0070700800248 W. J. Feng E. Pan X. Wang J. Jin Rayleigh waves in magnetoelectroelastic half planes Received: 23 August 2007 / Revised: 17 February 2008 /
More information(This is a sample cover image for this issue. The actual cover is not yet available at this time.)
(This is a sample cover image for this issue. The actual cover is not yet available at this time. This article appeared in a journal published by Elsevier. The attached copy is furnished to the author
More informationJ. Sladek, V. Sladek & M. Hrina Institute of Construction and Architecture, Slovak Academy of Sciences, Bratislava, Slovakia
Evaluation of fracture parameters for functionally gradient materials J. Sladek, V. Sladek & M. Hrina Institute of Construction and Architecture, Slovak Academy of Sciences, 842 20 Bratislava, Slovakia
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationThe ElasticViscoelastic Correspondence Principle for Functionally Graded Materials, Revisited
S. Mukherjee ASME Fellow Department of Theoretical and Applied Mechanics, Cornell University, Kimball Hall, Ithaca, NY 14853 email: sm85@cornell.edu Glaucio H. Paulino 1 Mem. ASME Department of Civil
More informationModeling of Variable Lamé s Modulii for a FGM Generalized Thermoelastic Half Space
75 Modeling of Variable Lamé s Modulii for a FGM Generalized Thermoelastic Half Space Abstract In this work we consider a problem in the contet of the generalized theory of thermoelasticity for a half
More informationFinite element analysis of longitudinal debonding between fibre and matrix interface
Indian Journal of Engineering & Materials Sciences Vol. 11, February 2004, pp. 4348 Finite element analysis of longitudinal debonding between fibre and matrix interface K Aslantaş & S Taşgetiren Department
More informationM. Vable Mechanics of Materials: Chapter 5. Torsion of Shafts
Torsion of Shafts Shafts are structural members with length significantly greater than the largest crosssectional dimension used in transmitting torque from one plane to another. Learning objectives Understand
More informationA Study of Annular Plate Buckling Problem with Tension Loaded at Inner Edge
ANALELE UNIVERSITĂłII EFTIMIE MURGU REŞIłA ANUL XVII, NR. 1, 010, ISSN 14537397 Syed Noh, Mostafa Abdalla, Waleed Fekry Faris A Study of Annular Plate Buckling Problem with Tension Loaded at Inner Edge
More informationa x Questions on Classical Solutions 1. Consider an infinite linear elastic plate with a hole as shown. Uniform shear stress
Questions on Classical Solutions. Consider an infinite linear elastic plate with a hole as shown. Uniform shear stress σ xy = T is applied at infinity. Determine the value of the stress σ θθ on the edge
More informationEFFECTS OF THERMAL STRESSES AND BOUNDARY CONDITIONS ON THE RESPONSE OF A RECTANGULAR ELASTIC BODY MADE OF FGM
Proceedings of the International Conference on Mechanical Engineering 2007 (ICME2007) 2931 December 2007, Dhaka, Bangladesh ICME2007AM76 EFFECTS OF THERMAL STRESSES AND BOUNDARY CONDITIONS ON THE RESPONSE
More informationIntegral equations for crack systems in a slightly heterogeneous elastic medium
Boundary Elements and Other Mesh Reduction Methods XXXII 65 Integral equations for crack systems in a slightly heterogeneous elastic medium A. N. Galybin & S. M. Aizikovich Wessex Institute of Technology,
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationPSEUDO ELASTIC ANALYSIS OF MATERIAL NONLINEAR PROBLEMS USING ELEMENT FREE GALERKIN METHOD
Journal of the Chinese Institute of Engineers, Vol. 27, No. 4, pp. 505516 (2004) 505 PSEUDO ELASTIC ANALYSIS OF MATERIAL NONLINEAR PROBLEMS USING ELEMENT FREE GALERKIN METHOD Raju Sethuraman* and Cherku
More informationRadial Growth of a MicroVoid in a Class of. Compressible Hyperelastic Cylinder. Under an Axial PreStrain *
dv. Theor. ppl. Mech., Vol. 5, 2012, no. 6, 257262 Radial Growth of a MicroVoid in a Class of Compressible Hyperelastic Cylinder Under an xial PreStrain * Yuxia Song, Datian Niu and Xuegang Yuan College
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationSTRESS AND STRAIN ANALYSIS OF ROTATING FGM THERMOELASTIC CIRCULAR DISK BY USING FEM
International Journal of Pure and Applied Mathematics Volume 74 No. 3 2012, 339352 ISSN: 13118080 (printed version) url: http://www.ijpam.eu PA ijpam.eu STRESS AND STRAIN ANALYSIS OF ROTATING FGM THERMOELASTIC
More informationDiscrete Element Modelling of a Reinforced Concrete Structure
Discrete Element Modelling of a Reinforced Concrete Structure S. Hentz, L. Daudeville, F.V. Donzé Laboratoire Sols, Solides, Structures, Domaine Universitaire, BP 38041 Grenoble Cedex 9 France sebastian.hentz@inpg.fr
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationSmallScale Effect on the Static Deflection of a Clamped Graphene Sheet
Copyright 05 Tech Science Press CMC, vol.8, no., pp.037, 05 SmallScale Effect on the Static Deflection of a Clamped Graphene Sheet G. Q. Xie, J. P. Wang, Q. L. Zhang Abstract: Smallscale effect on the
More informationFatigue Damage Development in a Steel Based MMC
Fatigue Damage Development in a Steel Based MMC V. Tvergaard 1,T.O/ rts Pedersen 1 Abstract: The development of fatigue damage in a toolsteel metal matrix discontinuously reinforced with TiC particulates
More informationFurther Linear Elasticity
Torsion of cylindrical bodies Further Linear Elasticity Problem Sheet # 1. Consider a cylindrical body of length L, the ends of which are subjected to distributions of tractions that are statically equivalent
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationVIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS
VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,
More informationApplication of piezoelectric actuators to active control of composite spherical caps
Smart Mater. Struct. 8 (1999 18. Printed in the UK PII: S964176(9916614 Application of piezoelectric actuators to active control of composite spherical caps Victor Birman, Gareth J Knowles and John J
More informationEffect of Growth Direction on Twin Formation in GaAs Crystals Grown by the Vertical Gradient Freeze Method
Effect of Growth Direction on Twin Formation in GaAs Crystals Grown by the Vertical Gradient Freeze Method A.N. Gulluoglu 1,C.T.Tsai 2 Abstract: Twins in growing crystals are due to excessive thermal stresses
More informationNatural Boundary Element Method for Stress Field in Rock Surrounding a Roadway with Weak Local Support
Copyright 011 Tech Science Press CMES, vol.71, no., pp.93109, 011 Natural Boundary Element Method for Stress Field in Rock Surrounding a Roadway with Weak Local Support Shuncai Li 1,,3, Zhengzhu Dong
More informationFailure modes of glass panels subjected to soft missile impact
Failure modes of glass panels subjected to soft missile impact L. R. Dharani & J. Yu Dept. of Mech. and Aerospace Engineering and Engineering Mechanics, University of MissouriRolla, U.S.A. Abstract Damage
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationFinite element Analysis of thermo mechanical stresses of two layered composite cylindrical pressure vessel
Finite element Analysis of thermo mechanical stresses of two layered composite cylindrical pressure vessel Arnab Choudhury *1, Samar Chandra Mondol #2, Susenjit Sarkar #3 *Faculty, Mechanical Engineering
More informationJadavpur University, Kolkata
Finite Element Analysis of Transient Thermo Mechanical Stresses of Multilayered Composite Hollow Thick Cylindrical Pressure Vessel Arnab Choudhury 1, Samar Chandra Mondol 2, Susenjit Sarkar 3 1 Research
More informationMidterm Examination. Please initial the statement below to show that you have read it
EN75: Advanced Mechanics of Solids Midterm Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use two pages
More informationScienceDirect. Hamiltonian approach to piezoelectric fracture
Available online at www.sciencedirect.com ScienceDirect Procedia Materials Science 3 ( 014 ) 318 34 0th European Conference on Fracture (ECF0) Hamiltonian approach to piezoelectric fracture J.M. Nianga
More informationA note on finite elastic deformations of fibrereinforced nonlinearly elastic tubes
Arch. Mech., 67, 1, pp. 95 109, Warszawa 2015 Brief Note A note on finite elastic deformations of fibrereinforced nonlinearly elastic tubes M. EL HAMDAOUI, J. MERODIO Department of Continuum Mechanics
More informationPROPAGATION OF CURVED CRACKS IN HOMOGENEOUS AND GRADED MATERIALS
PROPAGATION OF CURVED CRACKS IN HOMOGENEOUS AND GRADED MATERIALS Abstract Matthew T. Tilbrook, Robert J. Moon and Mark Hoffman School of Materials Science and Engineering University of New South Wales,
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationCRACK INITIATION CRITERIA FOR SINGULAR STRESS CONCENTRATIONS Part I: A Universal Assessment of Singular Stress Concentrations
Engineering MECHANICS, Vol. 14, 2007, No. 6, p. 399 408 399 CRACK INITIATION CRITERIA FOR SINGULAR STRESS CONCENTRATIONS Part I: A Universal Assessment of Singular Stress Concentrations Zdeněk Knésl, Jan
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationINFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK BETWEEN THE TWO LAYERS
Djoković, J. M., et.al.: Influence of Temperature on Behavior of the Interfacial THERMAL SCIENCE: Year 010, Vol. 14, Suppl., pp. S59S68 S59 INFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationFrontiers of Fracture Mechanics. Adhesion and Interfacial Fracture Contact Damage
Frontiers of Fracture Mechanics Adhesion and Interfacial Fracture Contact Damage Biology, Medicine & Dentistry The Next Frontiers For Mechanics One of the current challenges in materials & mechanics is
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationFigure 21: Stresses under axisymmetric circular loading
. Stresses in Pavements.1. Stresses in Fleible Pavements.1.1. Stresses in Homogeneous Mass Boussinesq formulated models for the stresses inside an elastic halfspace due to a concentrated load applied
More informationThermal loadinduced notch stress intensity factors derived from averaged strain energy density
Available online at www.sciencedirect.com Draft ScienceDirect Draft Draft Structural Integrity Procedia 00 (2016) 000 000 www.elsevier.com/locate/procedia 21st European Conference on Fracture, ECF21, 2024
More informationPEAT SEISMOLOGY Lecture 2: Continuum mechanics
PEAT8002  SEISMOLOGY Lecture 2: Continuum mechanics Nick Rawlinson Research School of Earth Sciences Australian National University Strain Strain is the formal description of the change in shape of a
More informationAn Analytical Model for Long Tube Hydroforming in a Square CrossSection Die Considering Anisotropic Effects of the Material
Journal of Stress Analysis Vol. 1, No. 2, Autumn Winter 201617 An Analytical Model for Long Tube Hydroforming in a Square CrossSection Die Considering Anisotropic Effects of the Material H. Haghighat,
More informationFinite Element Modeling of Residual Thermal Stresses in FiberReinforced Composites Using Different Representative Volume Elements
Proceedings o the World Congress on Engineering 21 Vol II WCE 21, June 3  July 2, 21, London, U.K. Finite Element Modeling o Residual Thermal Stresses in FiberReinorced Composites Using Dierent Representative
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Thermodynamics Derivation Hooke s Law: Anisotropic Elasticity
More informationMECHANICS OF MATERIALS
GE SI CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes: J. Walt Oler Texas Tech University Torsional Loads on Circular Shafts
More informationElastic plastic bending of stepped annular plates
Applications of Mathematics and Computer Engineering Elastic plastic bending of stepped annular plates JAAN LELLEP University of Tartu Institute of Mathematics J. Liivi Street, 549 Tartu ESTONIA jaan.lellep@ut.ee
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationA modified quarter point element for fracture analysis of cracks
ndian Journal of Engineering & Materials Sciences Vol. 14, February 007, pp. 3138 A modified quarter point element for fracture analysis of cracks Sayantan Paul & B N Rao* Structural Engineering Division,
More informationOn the uniformity of stresses inside an inhomogeneity of arbitrary shape
IMA Journal of Applied Mathematics 23) 68, 299 311 On the uniformity of stresses inside an inhomogeneity of arbitrary shape Y. A. ANTIPOV Department of Mathematics, Louisiana State University, Baton ouge,
More informationVibroacoustic response of FGM plates considering the thermal effects Tieliang Yang1, a, Qibai Huang1, *
3rd International Conference on Materials Engineering, Manufacturing Technology and Control (ICMEMTC 2016) Vibroacoustic response of FGM plates considering the thermal effects Tieliang Yang1, a, Qibai
More informationLinear Elastic Fracture Mechanics
Measure what is measurable, and make measurable what is not so.  Galileo GALILEI Linear Elastic Fracture Mechanics Krishnaswamy RaviChandar Lecture presented at the University of Pierre and Marie Curie
More informationInternational Journal of Engineering Science
International Journal of Engineering Science 63 (2013) 1 9 Contents lists available at SciVerse ScienceDirect International Journal of Engineering Science journal homepage: www.elsevier.com/locate/ijengsci
More informationSettlement analysis of viscoelastic foundation under vertical line load using a fractional KelvinVoigt model
Geomechanics and Engineering, Vol. 4, No. 1 (01) 6778 67 Technical Note Settlement analysis of viscoelastic foundation under vertical line load using a fractional KelvinVoigt model HongHu Zhu* 1, LinChao
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More information